High performance ozone based advanced oxidation processes catalyzed with novel argon plasma treated iron oxyhydroxide hydrate for phenazopyridine degradation

The present study has focused on the degradation of phenazopyridine (PhP) as an emerging contaminant through catalytic ozonation by novel plasma treated natural limonite (FeOOH·xH2O, NL) under argon atmosphere (PTL/Ar). The physical and chemical characteristics of samples were evaluated with different analyses. The obtained results demonstrated higher surface area for PTL/Ar and negligible change in crystal structure, compared to NL. It was found that the synergistic effect between ozone and PTL/Ar nanocatalyst was led to highest PhP degradation efficiency. The kinetic study confirmed the pseudo-first-order reaction for the PhP degradation processes included adsorption, peroxone and ozonation, catalytic ozonation with NL and PTL/Ar. Long term application (6 cycles) confirmed the high stability of the PTL/Ar. Moreover, different organic and inorganic salts as well as the dissolved ozone concentration demonstrated the predominant role of hydroxyl radicals and superoxide radicals in PhP degradation by catalytic Ozonation using PTL/Ar. The main produced intermediates during PhP oxidation by PTL/Ar catalytic ozonation were identified using LC–(+ESI)–MS technique. Finally, the negligible iron leaching, higher mineralization rate, lower electrical energy consumption and excellent catalytic activity of PTL/Ar samples demonstrate the superior application of non-thermal plasma for treatment of NL.

species, which is capable to oxidize the most of refractory compounds to more biodegradable and less toxic intermediates 14 . Both heterogeneous and homogenous catalytic ozonation processes were applied; however, the heterogeneous processes is more favorable because of the simplicity of process, ease of catalyst separation and no secondary pollution 15 . Nevertheless, mass transfer resistance due to the particle size and few reaction sites are the main drawbacks of heterogeneous operation which can be solved by using nanostructured materials 16 . Numerous catalysts have been used in the literature including metal oxides, activated carbon, natural and synthetic materials [17][18][19][20][21] . The low-cost and abundant natural iron oxides are available in form of crystalline minerals such as goethite, ilmenite, limonite, magnetite and hematite 18 . Limonite is one of these minerals that is widely distributed around the globe. Natura limonite (NL) contains fine crystal grains from multiphase mixture with porous structure and large specific surface area as well as a high surface energy which results in a stronger capability. The salient property of NL that enhances its catalytic activity is the presence of superficial hydroxyl groups on its surface which participates in the production of hydroxyl radicals 22 . The modification of natural minerals is an effective way to increase their application, which is done using both physical and/or chemical processes. Mechanical modification is a simple, inexpensive and efficient method to reduce the size of minerals from micrometers to nanometers. Furthermore, chemical activation is effective to enhance surface hydroxyl groups as well as specific surface area 18,23 . From different types of modification methods, non-thermal plasma technique is one of the newest methods for surface modification. The main feature of plasma technology is environmentalfriendly, cost-effective, quickness, simplicity and ability of various nanostructures production 24 . Phenazopyridine hydrochloride (PhP) is a heterocyclic aromatic azo-compound that is used to help with the irritation, pain or urgency caused by urinary tract infections 25 . Due to the low water solubility (0.202 g/L) and low biodegradability, PhP accumulates in the sewages and therefore, treatment of PhP contaminated waters are very important 26 .
To the best of our knowledge, there is no comprehensive research on non-thermal glow discharge plasma method for treatment of NL in order to improve the structural properties and catalytic activity of this iron mineral. Different characterization analysis such as: FESEM, XRD, AAS, TEM, FTIR, BET-BJH, pH pzc and EDX confirmed the physical and chemical characteristics of synthesized samples. Moreover, in this research, the influence of the eco-friendly modified NL was evaluated by degradation of PhP antibiotic through catalytic ozonation process. For this purpose, the effect of main process parameters such as catalyst dosage, solution pH, initial contaminant and ozone concentration were investigated on the performance of process. In the following sections, the catalyst stability and reusability of as-prepared catalysts, Fe ions release, mineralization and also assessment of electrical energy consumption were also investigated. By evaluating the effect of organic and inorganic salts and also, the dissolved ozone concentration the PhP degradation mechanism was proposed. In addition the LC-( ESI)-MS/MS analysis used to recognize the produced intermediates and by-products during the PhP degradation by catalytic ozonation using PTL/Ar nanocatalysts. Only few reports have been worked on PhP oxidation intermediates in ozone based AOPs.

Materials and methods
Materials. NL ore was provided from Tekab iron mine (Est Azerbaijan, Iran). The PhP was used as pharmaceutical contaminant which characteristics are given in Table 1. Sodium thiosulfate (Na 2 S 2 O 3 .5H 2 O) as ozonation reaction quenching, sodium hydroxide (NaOH) and sulfuric acid (H 2 SO 4 ) for pH adjustment, potassium hydrogen phthalate (C 8 H 5 KO 4 , purity of 99.5%) for TOC calibration and, scavenging agents such as t-butanol (C 4 H 10 O), benzoquinone (BQ), sodium dihydrogen phosphate (NaH 2 PO 4 ), sodium carbonate (Na 2 CO 3 ) and sodium nitrate (NaNO 3 ) were provided from Merck Co. (Germany). Ultrapure water used for all experimental tests. All reagent used in the AOPs were pure and used as received without any purification.
Preparation of limonite nanostructures. The limonite nanostructures were produced from NL by nonthermal glow discharge plasma under argon atmosphere. The treatment procedure is schematically presented in Fig. 1. At first, NL samples were crushed by rod and ball milling to obtain microstructure particles. After sieving, washing with ultrapure water, filtration and drying at 70 °C, 3 g of the limonite was placed in a Pyrex tube plasma reactor, which was completely sealed with aluminum bonnets on both sides 12 . High-voltage direct current (DC) supplied by a DC power source was connected by the aluminum bonnets to generate glow discharge plasma. Argon gas with flowrate of 3 cm 3 /s was pumped within the reactor to bring the pressure to 50 Pa. The NL plasmatreated under Ar was denoted as PTL/Ar. www.nature.com/scientificreports/ Characterizations of limonites. The crystalline structure of NL and PTL/Ar samples were evaluated by X-ray diffraction (XRD) (Siemens D5000 diffractometer, 2θ = 10-80) armed with Cu-Kα (45 kV, 40 mA, λ = 1.54178 Å). The size and morphology of the NL and PTL/Ar samples were investigated using Field Emission. Scanning Electron Microscopy equipped with an EDX microanalysis (FESEM; DSM-960A Zeiss, Germany) and Transmission Electron Microscopy (TEM; LEO 912AB). Fourier Transform Infrared spectra (FTIR) were conducted in Bruker Tensor 27 (400-4000 1/cm). The specific surface area (S BET ), porosity, pore diameter and volume of NL and PTL/Ar samples were calculated by physical nitrogen adsorption and desorption experiment (at 77 K and room temperature, respectively) using Brunauer Emmett Teller (BET) analysis (ChemBET3000, USA). The Microstructure Distance Measurement software was used to evaluate particle size distribution of the nanoparticles (Nahamin Pardazan Asia Co., Iran). The atomic absorption spectroscopy (AAS) analyses measured the concentration of Fe ions released in the aquatic medium (Novaa 400 Analytikjena). The point of zero charge (pH PZC ) was performed by a procedure proposed by Mustafa et al. 27 . In this method, ten glass bottles containing 40 mL NaNO 3 (0.1 M) in ultrapure water with different pH values between 2 and 11 were prepared, each bottles containing 0.2 g of NL or PTL/Ar. The suspensions stirred for 48 h at 25 ℃. The pH PZC is defined by plotting the final pH versus initial pH.

Ozone based advanced oxidation processes experiments. Semi-batch experiments of ozonation
based processes were performed in a tubular Pyrex reactor with 4 cm internal diameter and 35 cm in height, as illustrated in Fig. 2. Ozone was generated using Ozomatic ozone generator (Germany) and through a diffuser entered to the reaction medium. In each experiment, 250 mL solution was prepared containing desirable concentration of PhP between 30 and 60 mg/L and, catalyst dosage between 0.25 and 1 g/L in deionized water. Afterward, the solution was treated by chosen different ozone concentration between 7 and 15 mg/L. At different time of reactions samples were taken from the reactor and quenched immediately with Na 2 S 2 O 3 (0.01 M). Then, filtered by a 0.45 µm PTFE filter for further analysis.
Analytical methods. The concentration of PhP at different times of reaction was evaluated at 270 nm through a UV-Vis spectrophotometer (WPA Lightwave S2000, UK). A VCSH TOC analyzer (Shimadzu, Japan) was conducted to measure the Total organic carbon (TOC) of samples. The residual ozone concentration in the solution was evaluated by Indigo colorimetric procedure 28 .
The degradation percent of PhP and TOC removal were calculated using Eq. (1) where M 0 (mg/L) and M t (mg/L) are the concentration/TOC at initial and t (min) time of concentration, respectively. www.nature.com/scientificreports/ larger contacting interfaces of α-FeOOH nanocatalysts consequently, the mass transport limitations could be lower compared to non-treated samples. As the results indicated an improvement in morphological characteristics of limonite samples was observed after plasma-treatment. Moreover, it can be said the smaller particle size, higher porosity and the rough structure of plasma treated samples will increase the catalytic activity of PTL/Ar. EDX, TEM and particle size distribution. The results of EDX analysis for the samples before and after plasma treatment were shown in Fig. 5a,b, respectively. The inset tables of these graphs showed the presence of Fe, O, C and Si in higher amounts which indicated the purity of the precursors. Moreover, these results proved the presence of elements were not changed before and after plasma treatment. On the other hand, the plasma treatment increased the Fe atoms in the surface of nanocatalysts. It can be clearly seen that by increasing the intensity of the Fe peaks the intensity of C peak in the treated samples were decreased. As a consequence of this reduction the surface of treated samples made free of carbon impurities. Further studies on PTL/Ar surface morphology were performed by TEM analysis and the micrograph was shown in Fig. 5e. For detailed analysis, Fig. 5c,d,f illustrated the diameter size distribution of particles on the surface of PTL/Ar derived from FESEM and TEM micrographs. The as prepared nanocatalyst has a narrow size distribution. Accordingly, all particles were less than 28 nm in diameter size. Also, the major portion of the particles is in the range of 15-17 nm (37.5%).
FTIR. The FT-IR spectra of both NL and PTL/Ar samples in the range of 400-4000 cm −1 are shown in Fig. 6.
In both natural and treated samples, adsorption bonds around 1640 and 3420 cm −1 can be related to O-H bond in water molecules 29 . Also, the peak around 3650 cm −1 is assigned to OH-groups 30 . The peaks in the range of 1542 and 1640 cm −1 can be related to vibration mode of the C-H bond 29,31 . The peaks in 1732 cm −1 region are associated with the C=O vibrations. The peaks at about 537 and 471 cm −1 may be related to the tensile vibrations of the Fe-O bond. Furthermore, the absorption bands at around 792, 901 and 1024 cm −1 are also related to the stretching mode of the surface Fe-OH groups, which are the most important factor in the formation of surface hydroxyl groups 12 . A significant increase in the intensity of Fe-related peaks is observed in the plasma-treated sample. This phenomenon can be related to the increase in purity as well as the increase in surface iron after plasma processing. In addition, the vibrations at 792, 901, and 1024 cm −1 also related to Fe-OH surface groups which significantly increased by plasma treatment. Also, the location of the available peaks is similar for both samples which confirm that the surface functional groups are the same for NL and PTL/Ar samples.
Textural properties. BET-BJH analysis was performed for determination of the specific surface area, pore diameter and volume of the raw and treated samples. Figure 7a,b, presented the pore size distribution and N 2 adsorption-desorption isotherms for NL and PTL/Ar. As it is obvious both samples showed Type-IV isotherm behavior (ISO 15,901-2) with a hysteresis cycle, revealing the porous structure with meso-micro cavities. The obtained results also indicated that the closed pores converted to interconnected open cavities. Also, the H4 type hysteresis can be considered for limonite samples, indicating narrow gap cavities. The textural properties of NL and PTL/Ar including total pore volume, pore diameter and specific surface area are listed in Table 2. From Ar adsorption/desorption experiment, limonite has a surface area of 33.37 m 2 /g which increased to 49.16 m 2 /g after plasma treatment. The pore volume of PTL/Ar samples was obtained about 0.039 cm 3 /g which improved significantly compared to NL samples (0.023 cm 3 /g) as a consequence of plasma treatment. This increase in www.nature.com/scientificreports/    www.nature.com/scientificreports/ specific surface area results in the generation of more active sites on the surface of the catalyst and consequently, enhances the performance of catalytic process.
pH PZC determination. The pH PZC was determined by plotting the final pH versus the initial pH. As depicted in Fig. 8, the pH PZC of the NL and PTL/Ar were measured 6.4 and 6.7, respectively, indicating successful hydroxylation of limonite after Ar-plasma treatment. The net surface charge of limonite is zero at pH PZC . Furthermore, the surface of limonite positively charged when pH solution < pH PZC and negatively charged when pH solution > pH PZC 32 . According to Eq. (3), the protonation of limonite happened when pH of solution was lower than 6.4 and, deprotonation was happened when pH of solution was higher than 6.4, according to Eq. (4) 12 .
Oxidation process. Effect of different oxidation processes. The degradation of PhP was evaluated in the absence and presence of ozonation. Figure 9 shows the comparison of PhP degradation with different processes including adsorption with NL and PTL/Ar, ozonation, catalytic ozonation using NL and PTL/Ar. As can be seen from this figure, the adsorption of PhP was 12% on PTL/Ar and 8% on NL after 40 min of treatment. A little increase in PhP degradation through adsorption on PTL/Ar is attributed to the nanostructured limonite formation under plasma treatment which increased the specific surface area. In the oxidation processes, O 3 /PTL/Ar showed the most efficient process. The degradation of PhP reached to 58%, 77% and 97% through O 3 , O 3 + NL and O 3 + PTL/Ar, respectively. A sharp increase in PhP degradation in the O3 + PTL/Ar process indicated good capability of this process toward generation of reactive species. The catalytic performance of limonite is defined by two mechanisms: 1-presence of hydroxyl groups on the surface and, 2-presence of iron ions in the limonite structure 33 . The interaction of ozone and surface hydroxyl groups make a series of chain reactions which causes to formation of reactive species specially hydroxyl radicals. The proposed mechanism for ozone decomposition on PTL/Ar surface can be described as Eqs. (5)-(10) 34 . www.nature.com/scientificreports/ Furthermore, plasma removes some impurities and more iron is available on the surface of limonite after plasma treatment 33 .
Moreover, the kinetic study of PhP degradation was studied. From Table 3 pseudo first order kinetics behavior of PhP degradation can be indicated for different processes. Adsorption on NL and PTL/Ar processes had the lowest apparent PhP degradation rate constants of 0.0026 and 0.0040, respectively. In contrast, the O 3 + PTL/ Ar process had the highest reaction rate constant due to synergistic effect between ozonation and adsorption processes. The synergic factor can be calculated from Eq. (11): The rate constants of adsorption by PTL/Ar and sole ozonation processes were 0.004 min −1 and 0.0219 min -1 , respectively, while for O 3 + PTL/Ar process was 0.0936 min −1 . Consequently, the synergy factor value was 11) synergy factor = k ′ catalytic ozonation k ′ adsorption + k ′ ozonation  www.nature.com/scientificreports/ calculated at 3.71 which mean significant enhancement was occurred through combination of processes. Fathinia et al. 35 also reported synergy factor for photocatalytic ozonation of PhP by TiO 2 coated on ceramic plates. As can be seen in Table 3 the highest synergy factor was reported about 2.11 for PhP degradation at the optimized operating condition which is lower than synergy factor of O 3 + PTL/Ar process. This can be explained by higher ROSs generation in presence of PTL/Ar in ozonation process. As a result, O 3 + PTL/Ar process was selected as the desired catalyst for further catalytic ozonation experiments.
Effect of initial PhP concentration. Figure 10a displayed the effect of initial contaminant concentration on the degradation of PhP in the O 3 + PTL/Ar process. Experiments were performed at constant PTL/Ar dosage (0.75 g/L), ozone concentration (11 g/L), pH value (6.7) but at different initial PhP concentrations of 30, 40, 50 and 60 mg/L. The degradation of PhP was decreased from 98 to 71% by increasing its initial concentration from 30 to 60 mg/L, respectively. The degradation efficiency of PhP depends on the rate of radical generation. Whiles the oxidant concentration is constant, a competition occurred between the generated intermediates and byproducts with parent pollutant in reacting with radicals at high initial pollutant concentration 36 . Therefore, the possibility of ROSs reaction with PhP molecules decreases, which leads to reduction in degradation efficiency of oxidation process. A similar phenomena was observed by Khataee et al. 37 that the degradation of textile dye in the sono-Fenton/pyrite process was decreased as initial dye concentration increased.
Effect of initial pH. The initial pH of solution is one of the significant parameters in the heterogeneous processes. It was stated in the literature that the oxidation process conducted mainly near or on the surface of catalyst due to the short life-time of free radicals. Therefore, it is desirable that the contaminant not repelled but attracted to the surface. Considering the pK a of PhP (5.05) and pH PZC of nanocatalysts (6.7), so in the acidic condition both PhP repelled from the surface. In such condition the surface charge density of the nanocatalyst become positive while the PhP molecules are in cationic form thus an electrostatic repulsion forces occurred.
On the other hand, in the alkaline condition the negative charge density of surface and anionic form of PhP molecules hinder the contaminant adsorption and consequent reactions. In the moderate pH as Fig. 10b shows in the moderate pH value (6.7) the most effective PhP degradation was observed. In this pH value the surface Effect of catalyst dosage. The influence of catalyst loading on the performance of oxidation process is demonstrated in Fig. 10c. As depicted, the degradation efficiency of PhP increased as the initial catalyst dosage ranged from 0.25 to 1 g/L due to the enhancement in active sites and accordingly, more radical were generated on the surface of nanocatalyst 9 . However, no significant difference was observed in the degradation efficiency of PhP between catalyst dosages of 0.75 and 1 g/L. Therefore, 0.75 g/L was selected as the optimum dosage of PTL/Ar nanocatalysts for further experiments. In the similar study conducted by Liu et al. 38 , no noticeable difference was observed for degradation of p-nitrophenol when limonite dosage changed from 2 to 4 g/L.
Effect of initial ozone concentration. The effect of initial ozone concentration was evaluated over the range of 7-13 mgO 3 /L at constant pH, PhP concentration and catalyst dosage of 6.7, 30 mg/L and 0.75 g/L, respectively and the results are presented in Fig. 10d. The results showed that the degradation efficiency raised from 77 to 99% as ozone concentration increased from 7 mg/L to 13 mg/L. A direct relation between pollutant degradation efficiency and initial ozone concentration is attributed to the production of more reactive species specially hydroxyl radicals 33 . It should be noted that the final PhP degradation was the same in the experiments containing 11, 13 and 15 mgO 3 /L. Therefore, 11 mg/L ozone concentration was selected as optimum value for further experiments.
Stability and reusability. The stability of catalyst plays an important role in the long-term operation. For this purpose, the Fe content released in the solution was analyzed before and after oxidation process by AAS analysis. The results of Fig. 11a showed that 0.170 mg/L and 0.048 mg/L Fe ions were detected in the O 3 + NL and O 3 + PTL/Ar processes, respectively. Therefore, the plasma treatment significantly decreased the amount of Fe release to the reaction medium. The improvement in catalyst stability after plasma treatment also was reported by researchers 24,37 . In order to investigate the reusability of the catalyst, the performance of PTL/Ar after 6 runs was evaluated. The results of reusability study were illustrated in Fig. 11b. The efficiency of PhP degradation decreased from 98% in the first run to 89% in 6th run, indicating no noticeable loss was observed in the PTL/Ar TOC removal and electrical energy efficiency. The mineralization of PhP oxidation process was evaluated by measuring total organic carbon (TOC). As illustrated in Fig. 12 In this research, the electrical energy per order (E EO ) of the above processes was calculated using Eq. (12) as follows 40 : where P is the input power (kW) of the system, t is the process time (h), V is the volume of aquatic solution (L), TOC 0 (mg/L) and TOC f (mg/L) are the initial and final total organic carbons, respectively. The E EO values for degradation of PhP according to optimum condition were calculated and the results are shown in Fig. 12. However, it seems that the combined processes are not cost-effectiveness but according to Fig. 12a,b the O 3 + PTL/ Ar process had the lowest energy consumption as well as highest TOC removal compared to O 3 , O 3 + NL and O 3 + H 2 O 2 processes. Mehrjouei and co-workers 11,41 compared the economic aspects of photocatalytic oxidation, photo and catalytic ozonation processes for degradation of dichloroacetic acid and oxalic acid and reported that photocatalytic ozonation represented the highest cost-effectiveness between the investigated processes.
Elucidating the possible reaction mechanism of PhP degradation in catalytic ozonation. Scavenging study. Figure 13a www.nature.com/scientificreports/ ated radicals instead of reacting with PhP. From Fig. 13a, almost complete PhP degradation was happen in the blank condition. In the experiment containing BQ, a decline in PhP degradation to 60% is noticed due to the high reactivity of TBA with hydroxyl radical. In the presence of TBA, strict scavenging was happened and, the degradation efficiency of PhP was reduced to 38%. The inhibitory effect of scavengers revealed that there are a few superoxide radicals in the system and, it was concluded that the hydroxyl radical was the main responsible for PhP degradation. The PhP degradation efficiency was decreased by addition of anionic salts to the solution medium (Fig. 13b,d). These anionic ions adsorbed on the PTL/Ar surface and occupied the surface active sites. Furthermore, the produced radicals can be consumed by the mentioned anions according to Eqs. (13)-(15) 9 : Therefore, the rate of radical production was decreased due to the presence of the salts and, carbonate had the greatest effect.
Dissolved ozone concentration and inorganic nitrogen evaluation. The concentration of dissolved ozone was evaluated during ozonation and catalytic ozonation (with PTL/Ar) processes and shown in Fig. 14a. As can be seen in sole ozonation process the concentration of dissolved ozone was improved significantly and then reached to about 2 mg/L in 40 min. On the contrary in the catalytic ozonation with PTL/Ar lower dissolved ozone concentration was observed and after 30 min of process the changes were very negligible. The lower dissolved ozone concentration means higher portion of ozone molecules was decomposed. As a consequence of ozone decomposition the reactive oxidative species will be generated in the medium and hence the PhP degradation will be increased. The higher dissolved ozone concentration in the presence of Fe-based natural catalysts was also reported in previous works 12,42 . The release of inorganic ions (NO 3 − and NO 2 − ) from N heteroatoms as a consequence of PhP bond cleavage in sole and catalytic ozonation is presented in Fig. 14b. As it can be seen www.nature.com/scientificreports/ NO 3 − and NO 2 − ions were accumulated in the medium gradually from the beginning of processes. More nitrate ions were created in both processes compared to nitrite ions. Nitrite ion concentration increased at beginning of processes and followed by a gradual decrease which can be due to conversion to nitrate. Nitrate ions were formed in a more extent in comparison with nitrite and the concentration was increased over time of reaction. Furthermore, the amount of NO 3 − and NO 2 − ions release was higher in O 3 + PTL/Ar process than sole O 3 . This means ozonation process in the presence of PTL/Ar nanocatalysts had more degradation efficiency compared to ozonation process alone. These findings are in consistence with the other researcher coutcomes 43 .
Analysis of PhP degradation intermediates and products. The produced intermediates and by-products PhP degradation during catalytic ozonation by PTL/Ar was evaluated by LC-MS analysis. The detected oxidation intermediates are summarized in Fig. 15. According to the obtained results, the attack of hydroxyl radicals to the PhP molecule (m/z = 214) can produce intermediate with m/z = 125 (2,3,6-Triaminopyridine) as the result of N = N band cleavage. In addition the "A intermediate (m/z = 215) can be produced as a result of · OH attack to N atom of amine group of PhP. 2,3,6-Triaminopyridine (A) degraded to 3-hydroxy-2,6-diaminopyridine with m/z of 126 which can furthered degraded to 2,6-diaminopyridine (m/z = 110). The intermediate with m/z of 124 ("B) was identified as a result of N=N bond cleavage of "A structure. Phenol compound (m/z = 95) was generated due to hydroxylation of "B bonds. Finally, multiple hydroxylation reactions and bond cleavage occurred and further reaction of · OH and other ROSs with different structures led to production of end-products such as H 2 O, CO 2 , and N ions.

Conclusions
In the present research, the beneficial limonite nanocatalysts were prepared by non-thermal glow discharge plasma under Ar atmosphere. Based on the characterization analyses, the small particle size, highly porous and rough nanostructure of plasma treated samples will improve the PhP degradation. A comparison between different degradation processes demonstrated that catalytic ozonation with PTL/Ar due to the higher specific surface area and total pore volume led to 96.4% degradation and 74% mineralization during 40 and 120 min of process, respectively. The excellent properties of nanostructures which were achieved by plasma treatment enhanced the penetration of pollutant molecules and thus improved the catalytic activity of PTL/Ar. The optimum amount of pH value, catalyst loading, initial ozone and contaminant concentration were observed to be www.nature.com/scientificreports/ 6.7, 0.75 m/L, 11 mg/L and 30 mg/L, respectively. Lower Fe ion release in addition to high reusability and stability during the catalytic ozonation process with PTL/Ar can be due to strengthening of the crystalline structure after plasma treatment in comparison with raw samples. The mineralization and electrical energy consumption results revealed that, in contrast to the O 3 , peroxone and O 3 + NL processes, the O 3 + PTL/Ar process expressed the highest mineralization and lowest electrical energy consumption under the optimized conditions. The PhP degradation mechanism was explored by different inorganic and organic scavengers as well as O 3 concentration evaluation which proved that the indirect ozone attack was the dominant degradation pathway. The main intermediates during PhP oxidation by catalytic ozonation processes using PTL/Ar were identified using LC-MS technique. Considering the supreme activity and stability of the plasma treated nanocatalyst, it can be concluded that PTL/Ar has potential for further practical applications.
Received: 9 September 2020; Accepted: 17 December 2020 Figure 15. Proposed possible degradation pathways of PhP in catalytic ozonation processes using PTL/Ar.